Phase Transformation Studies af a Low Alloy Steel in the (a ®³) Phase phase transformation...
Embed Size (px)
Transcript of Phase Transformation Studies af a Low Alloy Steel in the (a ®³) Phase phase transformation...
Materials Research. 2010; 13(1): 113-117 © 2010
Phase Transformation Studies af a Low Alloy Steel in the (a + γ) Phase Region
Kenneth Kanayoa Alanemea*, Celestine Mondeb Kammab
aDepartment of Metallurgical and Materials Engineering, Federal Univeristy of Technology, Akure, Nigeria
bDepartment af Metallurgical and Materials Engineering, University of Lagos, Nigeria
Received: November 7, 2009; Revised: January 29, 2010
This research work describes a thermo mechanical investigation of a low alloy steel treated in the (a + γ) phase region. The aim is to develop a high tensile, ductile microstructure that could have a wide range of engineering applications. Recent advances in the area of precipitation, recrystallization mechanisms, and a / γ transformations provide strong background to this study. In a preliminary heat treatment, various microstructures (normalized and 450 °C tempered martensite structure) were produced and deformed to varying degrees. Subsequently, these microstructures were subjected to various intercritical temperatures (740 and 760 °C) for various times and a very high cooling rate. Light (optical) microscopic investigations were carried out to study the ensuing microstructures. Mechanical testing results (tensile and hardness values) were used to characterize the structures obtained. On analysis of the result, it was observed that well defined micro-duplex structures of ferritic and martensitic nature, possessing good combinations of strength and ductility were obtained.
Keywords: thermomechanical, recrystallization mechanisms, micro-duplex structures, mechanical testing, crystallographic transformations
Phase transformations in crystalline solids are widely used in the design of microstructures or alloy development. Iron has various al- lotropic forms - it is this unique metallurgical property that makes it so popular for phase transformation considerations. In thermomechani- cal operations, for example, the effects of deformation and heating temperatures are very vital, usually, the chronological sequence in which the various phases appear matters a lot. In the thermomechani- cal treatment of steels, various metallurgical reactions are known to take place in different orders, thereby making the overall mechanism difficult to analyse and control1,2.
In phase transformations involving carbon steels, it has been observed that problems of precipitation and recrystallization arise due to concurrent reactions taking place, mutually affecting each other. This problem is very prevalent during intercritical treatments, which are utilized to produce steel having a good combination of high strength and plasticity, due to the presence of the dual phases – ferrite and martensite. In this case precipitation and recrystallization processes compete with the a → γ transformation making it difficult to establish optimum treatment conditions to achieve the best com- bination of ferrite and austenite, which on quenching in water will yield the best synergy of strength and plasticity3. Hence meaningful engineering use derivable from the intercritical treatment has not been fully harnessed because of inconclusive comprehension of the transformation behaviour in the steel especially those of carbon content above 0.2 wt. (%) C.
The present work is a preface to the attempt to develop a high strength –ductile microstructure in a low alloy steel by studying the phase transformation behaviour during treatment in the intercritical phase region. The role of the treatment parameters (initial microstruc- ture, deformation, and temperature) will be well considered. Earlier
studies on recrystallization and precipitation phenomenon in carbon steels4 provide useful background to the test parameters.
2. Experimental Procedure
The equipment used for this research are lathe machine, milling machine, miniature cold rolling machine, muffle furnace, power hacksaw machine, metallographic mounting press, grinding and polishing machines, rockwell hardness tester, tensile testing machine, and optical microscope with camera.
The material used for this research was a low alloy steel with chemi- cal composition in wt. (%) as follows: C (0.4), Si (0.26), Mn (1.19), P (0.0419), S (0.0024), Cr (0.13), Ni (0.035), V(0.0017).
The material was first normalized to soften the steel for sub- sequent machining. The steel was austenitized at 860 °C for one hour, before cooling in air. Thereafter, the bulk sample was cut and machined to flat strips of thickness ranging from 2.5 to 10 mm.
2.3.1. Production of initial microstructure
As the metallurgical pre-history of the as-supplied, specimens were unknown; the machined specimens were initially normalized at 860 °C for 1 hour and then cooled in air, so as to restore the original condition and to induce homogeneity in the structure. After normal-
114 Alaneme & Kamma Materials Research
izing, different microstructures, serving as starting point-structures, were produced. The treatments were performed thus:
• Tempered Marten site™: M/450 °C, 1h/H 2 0.
• Five test pieces were soaked for 1hour at 860 °C and then quenched in water: 860 °C, 1h/H
2 0. The tempering of samples
was carried out at 450 °C for 1hour and then air-cooled. • Normalized (Pearlitic – feritic structure) P: 860 °C, 1h/air. Five test pieces which were earlier produced from the initial
normalization treatment were reserved for this purpose. Additionally, three frequently occurring steel microstructures –
here referred to as conventional steel microstructures were produced for the purpose of comparing properties with the structures produced after intercritical treatment. The structures produce are: normalized, martensite and 300 °C tempered martensite. These structures were produced in accordance with Alaneme5.
2.3.2. Thermomechanical treatment
The samples of different initial microstructures were all deformed to various degrees of 20, 35, 50, 70, and 80%. After the cold deforma- tion operation, the test pieces were subjected to intercritical heating
at temperatures of 740 and 760 °C for various times, ranging from 30 seconds to 60 minutes, before quenching in water.
2.3.3. Hardness measurement
The thermomechanically treated samples were subjected to hardness testing, using a Rockwell Hardness Tester. The hardness test was used to establish the different stages of transformation. The results of Hardness (HRB) Vs logarithm (base ten) of holding time is shown in Figures 1-4.
Microstructural characterization of the test specimens was per- formed using light miscroscopy. The specimen preparation for the light microscopy was conducted according to standard procedures6-8. The mechanisms of transformation (recrystallization and austenite/ ferrite reaction) as well as structural features were studied.
2.3.5. Tensile testing
Mechanical property characterization was done by the study of the tensile properties of selected microstructures obtained from
Figure 1. Photomicrograph showing the as-deformed microstructure of P/80%/760 °C. The structure reveals deformed pearlite (dark phase) and ferrite (white phase). The orientation of the ferrite indicates the direction of cold rolling. 400×.
Figure 2. Photomicrograph showing the microstructure of P/80%/760 °C, 1min/H
2 O. The structure reveals elongated pearlite (dark phase) and ferrite
(white phase). The ferrite grains are oriented along the direction of cold rolling. 400×.
Figure 3. Photomicrograph showing the microstructure of P/80%/760 °C, 15min/H
2 O. The structure reveals primary recrystallized grains of pearlite
and ferrite. 400×.
Figure 4. Photomicrograph showing the microstructure of P/80%/760 °C, 30 min/H
2 O. The structure reveals well defined duplex structure of ferrite
(white phase) and martensite (dark phase). The upper region shows that recrystallization is still in progress. 400×.
2010; 13(1) Phase Transformation Studies af a Low Alloy Steel in the (a+γ) Phase Region 115
the intercritical treatment and also the conventional steel heat- treatment. The tensile properties evaluated were the ultimate tensile strength and percentage elongation. The samples designation and corresponding treatment for the tensile test specimens are shown in Table 1.
3. Results and Discussion
Figure 1-5 are representative micrographs showing the microstructural evolution that occurs during intercritical treat- ment. It confirms that intercritical treatment develops micro- structures that exhibit micro-duplex features, made up of a ferritic zone combined with martensitic (formerly austenitic) zone ( Figures 4 and 5).
3.1.2. Rockwell hardness
The graphs of Hardness vs. log soaking time for the various starting-point microstructures and intercritical temperatures (740 and 760 °C) are shown in Figures 6-9. The curves have the following trend: First, a gradual fall in hardness (signifying recovery processes), second a further sharp fall showing that intense spheroidization and primary recrystallizaton process are dominant at this stage; thirdly, a sharp rise in hardness signifying the formation of increased amount of martensite; and finally a decrease in hardness indicating grain growth. Thus the general transformation